Nickel–carbon composite plating using a Watts nickel electroplating bath
- 141 Downloads
Metal–carbon composite platings have potential applications in various fields. We previously reported the preparation of nickel–nanocarbon composite platings using a Wood’s bath. The maximum carbon content was 1.2 mass%, but the maximum current efficiency of plating was 12%. The present study focuses on improving the current efficiency of the electroplating process used to prepare nickel–carbon black composites in a Watts bath contained carbon black. The microstructure and carbon content in the nickel plating were evaluated. The current efficiency was greater than 90%, but the carbon content of the composite plating layer was approximately 0.6 mass%. The incorporation of carbon black particles into the plating layer was influenced by the adsorption of particles onto the cathode surface, the supply of particles to the surface, and the electrodeposition rate. The carbon content in the plating layer was highest near the cathode surface and decreased with increasing thickness of the plating layer. The grain size of electrodeposits with carbon black was larger than that of deposits without carbon black. The space between grains was increased with increasing grain size. The corrosion resistance was diminished, indicating that the boundary was the originating point of corrosion.
KeywordsCarbonous nanomaterials Composite plating Wet process Electroplating
Nickel is an important element for surface treatment, and it is used to plate accessories, vehicle parts, and building materials. It can also coat resins and other organic materials via the electroless plating method, where it is typically deposited as a nickel–phosphorus alloy or nickel–boron alloy. In the electroplating method, a Watts bath is generally used for various applications and products. Meanwhile, a Wood’s bath is usually used when the substrate is stainless steel, nickel alloy, or other metals that form an oxide layer that inhibits the adhesion of materials. Composite plating is a useful technique that can increase the hardness, abrasion resistance, and lubricity through composite formation of a metal coating and fine particles of materials such as silicon carbide , alumina , boron nitride , and polytetrafluoroethylene [4, 5]. Carbon is a stable and highly conductive material. These composites are expected to exhibit both high corrosion resistance and good conduction. Carbon nanotubes, nanodiamond, and carbon black are the major reinforcement materials, and nickel–carbon composites have unique mechanical and electrical properties, especially high hardness, high elasticity, and a low widely adjustable friction coefficient for mechanical properties [6, 7, 8]. Applications for such composites have focused on hardness and thermal conductivity of carbon materials. On the other hands, utilization of electrical properties of carbon materials receives interest for electrode of battery and electromagnetic shielding materials [9, 10, 11, 12].
Several research groups have proposed and verified the co-deposition mechanism. A two-step adsorption process is one of the most widely accepted and useful mechanisms . In the case of nickel–carbon nanotube co-deposition, nickel was reduced on the ends and/or defects of carbon nanotubes and the deposits grew as spherical clusters of electrodeposited nickel . The surface character of the carbon materials was modified by certain processes such as hard treatment, plasma irradiation, mixed-acid cleaning, and dispersant addition [15, 16, 17, 18].
In a previous study, we produced a nickel–carbon black composite using a Wood’s bath. The carbon content reached 1.2 mass%, but the current efficiency was quite low . In the present study, we investigated the optimum condition and prepared a nickel–carbon black composite using galvanostatic electrolysis with a Watts bath for improving the current efficiency and surface morphology. Adsorption of the particles onto the surface, the supply of particles to the surface, and the reduction rate of metal on the surface are important factors in production of a composite layer during the plating process. The carbon content in the composite plating, surface morphology, and the corrosion resistance were also analyzed.
2 Materials and methods
A Watts-type bath containing 45 g L−1 nickel chloride hexahydrate, 240 g L−1 nickel sulfate, and 30 g L−1 boric acid was used as the electrolyte. The electrolyte pH was adjusted to 4.5 using sodium hydroxide. The carbon black was Vulcan XC 72R produced by CABOT. The carbon black was soaked in 10 vol% sulfuric acid solution to remove impurities. The purified carbon black was collected and rinsed with deionized water. It was ground in a mortar with a pestle after drying in an oven. The purified carbon black was added to the electrolyte, and the resultant mixture was sonicated for 30 min with an ultrasonic generator (VC-505, Sonics & Materials, Inc.) to improve the dispersion of carbon black in the electrolyte.
The electrodeposition of a nickel–carbon layer was performed in a glass cell with a volume of 200 cm3. The temperature of the electrolyte was maintained at 40 °C. The electrolyte was agitated with a magnetic stirrer. Control of the electroplating current, data collection, and data analysis were performed with a potentiostat/galvanostat (HZ5000, Hokuto Denko Corp.) connected to a personal computer. The working electrode (cathode) was a nickel plate, and the counter electrode (anode) was a Pt coil. The electrode area of the cathode was adjusted to 4 cm2 with PTFE tape (No. 903UL, Nitto Denko). The reference electrode was an Ag/AgCl electrode in saturated KCl solution; the electrolysis potential refers to the potential based on an Ag/AgCl electrode.
The surface morphology was observed by optical microscopy (OM, BH2-UMA, Olympus) and scanning electron microscopy (SEM, S-4800, Hitachi) equipped with an energy dispersive X-ray analyzer (EDS, X-Max80, HORIBA).
The corrosion resistance of the electroplating layer was determined by anodic polarization measurements in sulfuric acid solution at pH 3. The composite plating served as the working electrode (anode), and a Pt coil was used as the counter electrode (cathode). The scanning rate of the anodic polarization analysis was 2 mV s−1 from the rest potential. The corrosion potential was identified by the intersection of the tangent at 0.2 mA cm−2 of the anodic polarization curve with the line of 0 mA cm−2. For the anodic polarization measurements, the medium was deoxidized by Ar gas diffusion.
3 Results and discussion
3.1 Effect of carbon black concentration in electrolyte on carbon content in composite plating layer
In the process of electroplating, the carbon black particles must be adsorbed onto the cathode surface to be incorporated into the plating layer. In the case of a high concentration of carbon black in the electrolyte, although some adsorbed carbon black particles could be removed from the cathode surface to the electrolyte by agitation force, the concentration of carbon black particles in the electrolyte was sufficient to ensure adsorption onto the empty area of the cathode surface. The carbon content in the plating layer decreased with decreasing carbon black concentration in the electrolyte because the concentration of carbon black was insufficient to cover the cathode surface. Although the frequency of collision between carbon black particles on the cathode surface and particle in the electrolyte increased as the carbon black concentration in the electrolyte was increased, the incorporation of materials into the plating layer was balanced between the adsorption time of carbon black on the cathode surface and the metal electrodeposition rate. The carbon content was highest with small deviation at a carbon black concentration of 10 g L−1. Thus, we selected a carbon black concentration of 10 g L−1 for use in subsequent experiments.
3.2 Effect of agitation rate of the electrolyte on carbon content in composite plating layer
The carbon content varied greatly in experiments conducted without agitation. In the absence of agitation, the carbon black particles near the cathode surface were electrodeposited to the plating layer smoothly. However, the carbon black particles weakly interacted with the cathode surface and could be removed from the cathode surface by the force from the reductive reaction. In the case of agitation, the carbon black particles agglutinated with time. The carbon black particles on the cathode surface were agglutinated to a greater extent than the particles in suspension. Agglutinated carbon black incorporated into the plating layer would increase the carbon content, although carbon black aggregates were removed from the cathode surface easily. Therefore, the variation of the carbon content in the absence of agitation was greater than that observed under other conditions.
The aforementioned results suggest that carbon black was concentrated in the plating layer near the surface of the cathode. That is, when carbon black particles were adsorbed onto the cathode surface, some were buried in the plating layer. The carbon content in the plating layer decreased when the agitation rate was 500 rpm, suggesting that strong agitation could remove the carbon black from the cathode surface. On the contrary, at low agitation rates, insufficient carbon black was supplied to the surface, resulting in a low carbon content. On the basis of the aforementioned results, the agitation rate was fixed at 300 rpm in subsequent experiments.
3.3 Effect of plating thickness on carbon content in the composite plating layer
3.4 Effect of current density of plating on the carbon content in the composite plating layer
The current efficiency was approximately 60%, and a large amount of hydrogen gas was generated. Hydrogen gas generation can influence the generation of micropores in the plating, and the corrosion originates on the micropores of nickel plating. At low current density (< 10 mA cm−2), electrodeposited nickel did not bury the carbon black particles, and carbon black particles on the cathode surface were pushed into the electrolyte. The carbon black particles pushed from the cathode surface had electrodeposited nickel. Therefore, the current efficiency under the low-current-density condition was lower than that under other current-density conditions. A current density of 50 mA cm−2 was the optimum condition with respect to both the carbon content in the plating layer and the current efficiency.
3.5 Effect of carbon black on corrosion resistance and surface morphology
Carbon black does not influence the corrosion potential directly because it is a stable material under aqueous conditions. The coarsened grain increased the space between grains. The nickel–carbon plating was corroded from the space between grains; therefore, the corrosion potential of the nickel–carbon black plating was lower than that of the nickel plating without carbon black. At the beginning of electrodeposition, the cathode surface was covered by carbon black particles and the crystal cores of nickel metal were not produced in the interspaces among carbon black particles. The growth of grains was not inhibited by other grains in the nickel–carbon black plating. The grain size increased with increasing electroplating time until the grains contacted other grains. Therefore, the grain size of the nickel–carbon black plating was larger than that of the nickel plating without carbon black.
We prepared nickel–carbon black composite films using galvanostatic electrolysis with a Watts bath to study the factors that influence electroplating. The current efficiency was greater than 90% when using a Watts bath. However, the carbon content of the composite plating layer was approximately 0.6 mass%. The uptake of carbon black particles into the plating layer was influenced by the supply and adsorption of particles onto the cathode surface and by the electrodeposition rate. The carbon black was concentrated in the plating layer near the cathode surface. The corrosion resistance of the composite film decreased compared with that of a nickel plating layer without carbon black. The adsorption of carbon black particles onto the cathode surface resulted in larger electrodeposit grains and increased the space between grains, which was the originating point of corrosion.
Support of this work by “Knowledge Hub Aichi,” Priority Research Project and Aichi Prefecture Research, Development Subsidy from Aichi Prefectural Government, JSPS Core-to-Core Program, B. Asia-Africa Science Platforms and JST-OPERA Program (Grant Number: JPMOP1843.)
Compliance of ethical standards
Conflict of interest
The authors declares that they have no conflict of interests.
- 12.do Amaral MA, Marcuzzo J, Pinheiro BD, Lopes BHK, de Oliveira APS, Matsushima JT, Baldan MR (2019) Study of reflection process for nickel coated activated carbon fiber felt applied with electromagnetic interference shielding. J Mater Sci Technol 8:4040–4047Google Scholar
- 15.Chen Q, Dai L, Gao M, Huang S, Mau A (2001) Plasma activation of carbon nanotubes for chemical modification. J Phys Chem B 105:105618Google Scholar